**of flow-induced fiber orientation**

Kyeong-Hee Han and Yong-Taek Im^{a)}

*Computer Aided Materials Processing Laboratory, Department of Mechanical*
*Engineering, ME3227, Korea Advanced Institute of Science and Technology,*

*373-1 Kusong-dong, Yusong-gu Taejon 305-701, South Korea*
(Received 8 July 1998; final revision received 25 January 1999)

**Synopsis**

Distribution of fiber orientation in flow molding processes with short-fiber reinforcements is of
great importance because it affects the mechanical properties of molded parts. Due to trade-off
between the computational efficiency and accuracy, a second-order orientation tensor has been
widely used to describe the fiber orientation distribution. For calculation of this fiber orientation
tensor, a closure approximation has been introduced to reduce a higher fourth-order orientation
tensor to a lower second order. In the present investigation, a hybrid closure approximation has been
modified. Two parametric forms of the distribution function, which accurately describe the
random-in-space, random-in-plane, and uniaxial distributions of the fiber orientation were linearly
interpolated. The interpolating factor was obtained as a function of the fiber interaction coefficient
by fitting the distribution function calculations. Test simulation in homogeneous flow and
nonhomogeneous flow fields, respectively, showed that the proposed closure approximation gives
*good performance for a wide range of C*_{I}*values without showing nonphysical behavior. © 1999*
*The Society of Rheology.*@S0148-6055~99!01603-X#

**I. INTRODUCTION**

The fiber orientation distribution, which has a large effect on the mechanical proper- ties of the short-fiber-reinforced composite parts, greatly changes during processing. For effective production of such products via flow molding processes such as injection mold- ing and compression molding, it is essential to predict the flow-induced variation of the fiber orientation distribution. The importance of the distribution of such a fiber orienta- tion has led to many investigations.

Jeffery~1922! has derived the equation of orientation change of an ellipsoidal particle immersed in a homogeneous flow field based on hydrodynamics. Folgar and Tucker

~1984! have suggested a phenomenological model of rotary diffusivity to consider the change in orientation caused by fiber–fiber interactions. Since numerous short fibers exist in molded parts, it is impossible to consider fibers individually. Thus, the orientation distribution function~ODF!, which is a probability density function of the fiber orienta- tion, was introduced to fully describe the fiber orientation distribution in three dimen- sions. Adopting the ODF description in numerical simulations requires a tremendous amount of calculations since hundreds of degrees of freedom must be considered at each spatial point.

a!Author to whom all correspondence should be addressed. Electronic mail: ytim@convex.kaist.ac.kr

© 1999 by The Society of Rheology, Inc.

J. Rheol. 43~3!, May/June 1999 0148-6055/99/43~3!/569/21/$20.00 569

For more efficient numerical simulation of the orientation state of fibers, Advani and
Tucker ~1987! have made use of the orientation tensor which was originally introduced
by Hand~1962!. In this approach, only a few components are required to represent the
state of orientation at each spatial point. This advantage has allowed the orientation
tensor, especially the second-order tensor, to be widely used in the calculation of fiber
orientation in flow molding processes*@Altan et al. ~1990!; Bay and Tucker ~1992a,b!, de*
*Frahan et al.*~1992!; Gupta and Wang ~1993!; Ranganathan and Advani ~1993!; Tucker
and Advani~1994!; Chung and Kwon ~1995!; Ko and Youn ~1995!#. A weakness of the
orientation tensor approach is that a fourth-order tensor must be approximated by a
known second-order tensor in solving the governing equations. This closure approxima-
tion problem arises in many areas such as polymer dynamics and liquid-crystalline dy-
namics where the time evolution equation for the probability density is expressed in
terms of moments.

So far, the hybrid closure approximation proposed by Advani and Tucker~1987, 1990!

has most widely been used in the simulation of fiber orientations, since it is able to predict the trends of orientation distribution fairly well and can easily be implemented into numerical calculations. However, the involved numerical error is not negligible for some cases according to Bay and Tucker~1992b!. They concluded that for a quantitative agreement between simulations and experiments an improved closure approximation is required.

For this purpose, several approaches have been introduced. Bay ~1991! proposed a closure approximation based on the work by Hand~1962! by fitting steady-state orienta- tion distributions for a simple shear flow. Verley and Dupret~1993! proposed a natural closure approximation, a polynomial function of the second-order orientation tensor, which agrees with the analytic solutions of the ODF when assuming no fiber–fiber interactions. Cintra and Tucker~1995! proposed an orthotropic fitted closure approxima- tion in which three independent terms of the fourth-order orientation tensor were selected by assuming orthotropy. These terms were determined by fitting polynomial functions with numerical calculations of the ODF for selected flow fields. Schieber ~1993! and Chaubal and Leal ~1998! introduced parametric density estimation approach for micro- structured fluids in which a closure equation was constructed by proposing a parametric form of the ODF. This approach has an advantage over the previous curve fitting ap- proaches in that it automatically satisfies the important properties of the closure equation.

Considering the accuracy, however, it is less accurate than the fitting approach in general.

In the present investigation, both the parametric density estimation and the fitting approach were adopted to construct a new closure approximation in which two forms of the ODF were interpolated by applying the fitting with distribution function calculations.

This closure approximation accurately describes the random-in-space, random-in-plane, and uniaxial distributions of the fiber orientations, whereas the hybrid closure approxi- mation accurately describes the random-in-space and uniaxial distributions.

For verification, the predicted fiber orientation distribution using the second-order orientation tensor equation was compared to analytic and numerical solutions of the ODF. For numerical calculations of the ODF, finite-element formulations were carried out and calculations were performed using four different values of the fiber–fiber inter- action coefficient in various flow fields to ensure the generality and stability of the proposed closure approximation.

**II. FIBER ORIENTATION**

**A. Description of fiber orientation**

**The orientation of a single short fiber can be represented by the unit vector p shown in**
**Fig. 1. Components of the vector p are described by the angles**u ^{and}fas follows:

**p***5 ~p*1*, p*_{2}*, p*_{3}! 5 ~sinu^{cos}f^{, sin}u^{sin}f^{, cos}u!. ~1!

Describing the orientation by individual fibers is ineffective since composites contain numerous fibers which invoke difficulties in calculating the anisotropy induced by fiber orientation. Thus, the concept of probabilistic distribution is usually applied. The orien- tation distribution functionc is defined as a probability density function of fiber orien- tation as follows:

c**~p! 5**c~u^{,}f! [ lim
du^{,}df*→ 0*

*P*~u < u

### *

_{<}

_{u}

_{1}

_{du},

f<f

### *

_{<}

_{f}

_{1}

_{df})/~sinududf!. ~2!

From this definition, the ODF satisfies the following properties:

c**~p! 5**c**~2p!, or** c~u^{,}f! 5c~p2u^{,}p1f!, ~3!

15

### R

*S*c

**~p!dA 5**### E

u5 0 p### E

f5 02p

c~u^{,}f!sinu* ^{d}*f

*u*

^{d}^{,}~4!

*where, S denotes the surface of a unit sphere.*

In order to use the ODF description in numerical calculations, a great deal of effort is required to consider the ODF values in every direction at each spatial point. The orien- tation tensor, defined in the following manner, can greatly reduce such efforts:

second-order tensor: *a** _{i j}* 5

### R

*S*

*p*_{i}*p** _{j}*c

*~5!*

^{dA,}fourth-order tensor: *a** _{i j kl}*5

### R

*S*

*p*_{i}*p*_{j}*p*_{k}*p** _{l}*c

*~6!*

^{dA.}By definition, orientation tensors are symmetric in their indices and have the following normalized properties:

*a** _{kk}*5 1, ~7!

*a*_{ijkk}*5 a** _{ij}*, ~8!

where repeated indices indicate summation unless otherwise specified. These properties give the second-order orientation tensor five independent components to be considered.

**FIG. 1. Orientation of a single fiber described by the unit vector p.**

Thus, the second-order orientation tensor can effectively describe various fiber orienta-
tion distributions using minimum information. The fiber orientation distribution can be
visualized by using eigenvalues l*i* **and eigenvectors n*** ^{i}* of the second-order orientation
tensor as shown in Fig. 2.

**B. Rate of change of fiber orientation**

For description of the motion of a single fiber, all current models employ some form of the following equation:

*p˙** _{i}*5 21

2v*ij**p** _{j}*11

2l~g^{˙}*ij**p** _{j}*2g

^{˙}*kl*

*p*

_{k}*p*

_{l}*p*

*!2*

_{i}*D*

*c*

_{r}]c
]^{p}*i*

, ~9!

where v*i j* 5 ]^{v}*j*/]^{x}*i*2]^{v}*i*/]^{x}*j*, andg^{˙}*i j* 5 ]^{v}*j*/]^{x}*i*1]^{v}*i*/]^{x}*j* are components of the
vorticity and rate of deformation tensors, respectively, with ]^{/}]^{p}*i* being the gradient
operator on the surface of a unit sphere.l is a shape factor of the fiber particle defined as
*l [ (r*_{e}^{2}*21)/(r*_{e}^{2}11). As can be seen, it attains values between 0 ~sphere! and 1 ~infi-
nitely slender*!, depending on a function of the aspect ratio. D** _{r}*is the effective diffusivity

*that accounts for interactions among fibers. If D*

*5 0, Eq. ~9! becomes identical to Jeffery’s equation. In order to consider fiber–fiber interactions in nondilute suspensions,*

_{r}*Folgar and Tucker’s phenomenological model, D*

_{r}*5 C*

*I*g

*˙ , was used. In this model, C*

*is the interaction coefficient andg*

_{I}*5*

^{˙}### A

^{(}g

^{˙}*i j*g

^{˙}*i j*)/2 is an effective shear rate.

Regarding the rate of change of the ODF, the following continuity equation is ob- tained by assumingcto be a convected quantity:

*D*c

*Dt* 5 2 ]
]^{p}*i*

~c^{p˙}* _{i}*!, ~10!

*where, D/Dt denotes the material time derivative.*

Finally, taking the material time derivative of Eq.~5! and incorporating Eqs. ~9! and

~10!, the equation of change of the second-order orientation tensor can be obtained as
*Da*_{ij}

*Dt* 5 21

2~v_{ik}^{a}_{kj}*2a** _{ik}*v

*!11*

_{kj}2l~g^{˙}_{ik}^{a}_{kj}*1a** _{ik}*g

^{˙}*22g*

_{kj}

^{˙}

_{kl}

^{a}

_{ijkl}*!12C*

*g*

_{I}*~d*

^{˙}*ij*

*23a*

*!. ~11!*

_{ij}*To solve this equation, the fourth-order orientation tensor a** _{i j kl}*must be approximated as

*a function of the second-order orientation tensor a*

*. As can be intuitively sensed, this closure approximation has a critical effect on the solution accuracy of Eq.~11!.*

_{i j}**FIG. 2. Schematic representation of orientation distribution by the second-order orientation tensor.**

**III. CLOSURE APPROXIMATION**

The most frequently used closure approximation to date is the following hybrid clo- sure approximation~HYB! proposed by Advani and Tucker ~1987!:

*a*_{ijkl}^{HYB}*5 ~12 f !a*_{i j kl}^{LIN}*1 f a*_{i j kl}^{QUA}, ~12!

where

*a*_{ijkl}^{LIN}5 ^{1}7*~a**i j*d*kl**1a** _{ik}*d

*j l*

*1a*

*d*

_{il}*jk*

*1a*

*d*

_{kl}*i j*

*1a*

*d*

_{j l}*ik*

*1a*

*d*

_{jk}*il*!

235^{1}~d*i j*d*kl*1d*ik*d*j l*1d*il*d*jk*!, ~13!

*a*_{ijkl}^{QUA}*5 a*_{i j}*a** _{kl}*, ~14!

*and f* *5 1227 det(a**ij*).

This hybrid closure approximation accurately describes fiber orientation for random-in- space and uniaxial distributions and, in general, shows similar trends with the actual fiber orientation distribution observed in experiments. However, comparison with the distribu- tion function calculation shows that the involved error is not always negligible.

Since a closure approximation cannot exactly describe all situations of the fiber ori- entation distribution, it is important to select reference flow fields that will guarantee the smallest error for general cases of interest. In this investigation, a new closure approxi- mation is proposed for obtaining improved results of numerical calculations of the fiber orientation distribution during flow molding processes.

For simplification, the problem was considered in the principal coordinate system of
*a** _{i j}*. Ifl

*i*

**and n**

^{i}*5 (n*

_{1}

^{i}*,n*

_{2}

^{i}*,n*

_{3}

^{i}*) are the ith eigenvalue and is the ith eigenvector, respec-*

*tively, the second- and fourth-order orientation tensors denoted by b*

_{i j}*and b*

*can be represented in this coordinate system as follows:*

_{i j kl}*b*_{ij}*5 n*_{o}^{i}*n*_{p}^{j}*a** _{op}*5 l

*d*

_{i}*ij*,

*~no summation on i! and*~15!

*b*_{ijkl}*5 n*_{o}^{i}*n*_{p}^{j}*n*_{q}^{k}*n*_{r}^{l}*a** _{opqr}*. ~16!

Without loss of generality, the values ofl*i**(i* 5 1,2,3) lie in the shaded region of Fig.

3 with restriction of l1 > l2 > l3*. At the three extremity points R*_{s}*, R*_{p}*, and U, the*
eigenvalues become

**FIG. 3. Available region of eigenvalues in the**l11l21l35 1 plane.

*at R** _{s}*: l

_{1}5 l

_{2}5 l

_{3}5 1/3,

*at R*

*: l*

_{p}_{1}5 l

_{2}5 1/2, l

_{3}5 0, and

*at U:* l_{1}5 1, l_{2} 5 l_{3} 5 0. ~17!

*At R** _{s}*, various orientation distributions are possible, but in actual situations the most

*likely case is the random-in-space distribution. Similarly, R*

_{p}*and U were assumed to*represent random-in-plane and uniaxial distributions, respectively. These assumptions

*lead to the following nonzero components of b*

*at each extremity point:*

_{i j kl}*at R** _{s}*:

*b*

_{1111}

*5 b*

_{2222}

*5 b*

_{3333}

*5 1/5, b*

_{2233}

*5 b*

_{1133}

*5 b*

_{1122}5 1/15,

*at R*

*:*

_{p}*b*

_{1111}

*5 b*

_{2222}

*5 3/8, b*

_{1122}5 1/8, and

*at U:* *b*_{1111}5 1. ~18!

The main assumption of the current closure approximation to be applied to general cases of the fiber orientation distribution is that the conditions at these three extremities must be satisfied. This closure approximation will be defined as the modified hybrid closure approximation.

**A. Modified hybrid closure approximation: Model I**

The modified hybrid closure approximation, model I, was defined to satisfy Eq.~18!

by assuming the appropriate orientation distribution that exactly describes the conditions
at the three extremities. It is reasonable to expect the orientation distribution to be ex-
*pressed as simply as possible, e.g., egg like near R*_{s}*, disk like near R** _{p}*, and pen like near

*U. In this investigation, the following equations were assumed for each distribution:*

c^{egg}5 a_{1}^{r}_{1}^{2}1a_{2}^{r}_{2}^{2}1a_{3}^{r}_{3}^{2} ~a_{1} > a_{2} > a_{3} > 0!, ~19!

c^{disk}*5 ~12r*3

2!* ^{k}*~a

_{1}

^{r}_{1}

^{2}1a

_{2}

^{r}_{2}

^{2}

*! ~k > 0,*a

_{1}> a

_{2}> 0!, and ~20!

c^{pen}5 a_{1}*~12r*_{3}^{2}!^{k}*r*_{1}^{2m}*~k > 0, m > 1,* a_{1} > 0!, ~21!

*where r*_{i}**are components of the orientation vector p in the direction of n**^{i}*, and k, m, and*
a*i* *are parameters determined from a given a** _{i j}*. These ODFs are continuous in the
following sense:

c^{egg}u_{a}_{3}_{5 0}5 c^{disk}u_{k}_{5 0} and c^{disk}u_{a}_{2}_{5 0}5 c^{pen}u_{m}_{5 1}. ~22!

In fact, c^{pen} *can cover both disk- and egg-like regions if the condition of m* > 0 is
assumed. However, the combination of these three was employed since it is more physi-
cally meaningful and causes no notable differences in numerical results.

Since the ODF was defined to be symmetric in each coordinate plane, i.e., orthotropic,
*the fourth-order orientation tensor has six nonzero components, i.e., b*_{1111}*, b*_{2222}*, b*_{3333},
*b*_{1122}*, b*_{1133}*, and b*_{2233}*. Three of them, namely, b*_{1111}*, b*_{2222}*, and b*_{3333} and their
*eigenvalues can be calculated in terms of k, m, and*a*i*as shown in Table I. From this, the
relations between the second- and fourth-order orientation tensors can be derived as
follows:

Egg like (l3 > 1/5):

*b*_{1111}^{egg} 5 35^{3}~10l1*21!, b*_{2222}^{egg} 5 35^{3}~10l2*21!, and b*_{3333}^{egg} 5 35^{3}~10l321!.

~23!

Disk like (l3< 1/5, l1< 3l2!:

*b*_{1111}^{disk} 5 1*2s*

8 ~7l12l_{2}*!, b*_{2222}^{disk} 5 1*2s*

8 ~2l117l_{2}*!, and b*_{3333}^{disk} *5 ~3s!l*3,

*with s*5 l_{3}/~112l_{3}!. ~24!

Pen like (l_{3}< 1/5, l_{1}> 3l_{2}!:

*b*_{1111}^{pen} *5 ~12r!~12s!l*1, *b*_{2222}^{pen} *5 ~12s!l*2*2r~12s!l*1, *and b*_{3333}^{pen} *5 ~3s!l*3,
*with r* 5 l_{2}/~l113l_{2}*! and s 5 l*3/~112l3!. ~25!

Based on the normalized properties of Eq. *~8!, b*2233*, b*_{1133}*, and b*_{1122} can be deter-
mined as

*b*_{2233}*5 S2~l*1*2b*_{1111}*!, b*_{1133}*5 S2~l*2*2b*_{2222}*!, and b*_{1122}*5 S2~l*3*2b*_{3333}!,

~26!

*with S* *5 (12b*1111*2b*2222*2b*3333)/2.

Thus, the modified hybrid closure approximation, model I, can be defined based on the above results as

**TABLE I.** Principal components of the second- and fourth-order orientation tensors in terms of the parameters
in Eqs.~19!–~21!.

Egg like Disk like Pen like

ODF~c! a1*r*_{1}^{2}1a2*r*_{2}^{2}1a3*r*_{3}^{2} (1*2r*3

2)* ^{k}*(a1

*r*

_{1}

^{2}1a2

*r*

_{2}

^{2}) a1(1

*2r*3 2)

^{k}*r*

_{1}

^{2m}Normali- zation

15b11b2

154p

3 ~a11a21a3! b1[

### S

^{p}

^{E}

^{0}

^{p}

^{~}

^{sin}

^{f}

^{!}

^{2k}^{13}

^{d}^{f}

### D

^{a}

^{1}

^{1}

^{5}

### S ^{E}

^{0}

^{2}

^{p}

^{~}

^{cos}

^{u}

^{!}

^{2m}

^{d}^{u}

### D

•

### S ^{E}

^{0}

^{p}

^{~sin}

^{f}

^{!}

^{2k}

^{12m11}

^{d}^{f}

### D

^{a}

^{1}

b2[

### S

^{p}

^{E}

^{0}

^{p}

^{~}

^{sin}

^{f}

^{!}

^{2k}^{13}

^{d}^{f}

### D

^{a}

^{2}

l1 4p

15~3a11a21a3! *2k*14

4*~2k15!*~3b11b2! *~2m11!~2m12k12!*

*~2m12!~2m12k13!*

l2 4p

15~a113a21a3! *2k*14

4~2k15!~b113b2! *2m**12k12*

*~2m12!~2m12k13!*

l3 4p

15~a11a213a3! b11b2
*2k*15

1
*2m**12k13*

*b*_{1111} 4p

35~5a11a21a3! *~2k14!~2k16!*

8*~2k15!~2k17!*~5b11b2! *~2m11!~2m13!~2m12k12!~2m12k14!*

*~2m12!~2m14!~2m12k13!~2m12k15!*

*b*_{2222} 4p

35~a115a21a3! *~2k14!~2k16!*

8*~2k15!~2k17!*~b115b2! 3~2m12k12!~2m12k14!

*~2m12!~2m14!~2m12k13!~2m12k15!*

*b*_{3333} 4p

35~a11a215a3! 3~b11b2!

*~2k15!~2k17!*

3

*~2m12k13!~2m12k15!*

*a*_{ijkl}^{model I}[

## H

^{a}^{a}^{a}

^{i j kl}^{egg}

^{i j kl}^{disk}

^{i j kl}^{pen}

^{if}

^{if}

^{if}

^{l}

^{l}

^{l}

^{3}

^{3}

^{3}

^{> 1/5}

^{, 1/5,l}

^{, 1/5,l}

^{1}

^{1}

^{< 3l}

^{. 3l}

^{2}

^{2}

^{.}

^{~27!}

This equation is a continuous function ofl* _{i}*since it was based on a continuous ODF.

**B. Modified hybrid closure approximation: Model II**

As mentioned earlier, model I has an orthotropic property, and thus, is similar to the orthotropic closure approximation which was proposed by Cintra and Tucker ~1995!.

They have proposed two kinds of closure approximations. Orthotropic fitted closure

~ORF! is composed of polynomial functions of l*i* that were fitted to the numerical
*solutions of the ODF with C** _{I}*5 0.01 and l 5 1, and so, it does not explicitly satisfy the
conditions at the three extremities. On the other hand, orthotropic smooth closure~ORS!,
which is described below, is a linear interpolation of the three special cases represented
in Eq.~18!. In this sense, it can be considered to be a kind of modified hybrid closure.

*b*_{1111}^{ORS}5 20.1511.15l_{1}20.10l_{2},
*b*_{2222}^{ORS}5 20.1510.15l110.90l2, and

*b*_{3333}^{ORS} 5 0.6020.60l_{1}20.60l_{2}. ~28!

The above results can be obtained by assuming the following parametric form of the distribution function:

c^{ORS}**~r! 5** c^{ORS}~u

### *

,w### *

_{! 5}

^{b}

^{1}

4p^{1}
b2

2pd

### S

^{u}

^{*}

^{2}

^{p}

^{2}

### D

^{1}

^{b}

^{3}

^{d}

### S

^{u}

^{*}

^{2}

^{p}

^{2}

### D

^{d}

^{~}

^{w}

^{*}

^{!, ~29!}

where, u

### *

andw### *

**are the angles of r as in Eq.**~1! and d~•! is the delta function. The three parametersb1,b2, andb3can be easily obtained, respectively, from the definition of the orientation tensor as follows:

b15 3l_{3}, b25 2~l22l_{3}!, and b35 l_{1}2l_{2}. ~30!

ORS and model I have the following properties for alll*i*:

*b*_{1111}^{ORS} *. b*_{1111}^{model I}, *b*_{2222}^{ORS} *. b*_{2222}^{model I}, and *b*_{3333}^{ORS} *. b*_{3333}^{model I}. ~31!

This is evident from the definition of each distribution function. As will be discussed
*later, the b** _{i jkl}* values from the distribution function calculations ~DFC! generally lie
between those from model I and the ORS results. Therefore, a more accurate version of
the modified hybrid closure approximation, model II, can be defined by combining model
I and the ORS as

c^{model II}5 ~12FAC!•c^{model I}1FAC•c^{ORS}^{,} ^{or} ~32!

*a*_{ijkl}^{model II}*[ ~12FAC!•a**i j kl*
model I

*1FAC•a**i j kl*

ORS, ~33!

where FAC is an interpolating factor and can be determined by fitting the DFC results.

**IV. CALCULATION OF ODF**

In order to check whether the solution of Eq.~11! using the present modified closure approximation agrees with the exact solution of the orientation distribution, solutions of

the orientation distribution function are required. Hereafter, ‘‘exact solutions’’ or ‘‘exact values’’ will imply those obtained from the distribution function calculations. The mate- rial time derivative in Eq.~10! makes numerical calculations of the ODF nearly impos- sible if both space and time are considered. Therefore, in this investigation, exact solu- tions were calculated by analytic or numerical methods where material particles were followed in homogeneous flow fields.

**A. Analytic solution**

*When C** _{I}*5 0, an analytic solution of the ODF is available since the orientation vector

**p can be expressed in terms of an initial vector and a velocity gradient. Applying the**

*initial condition p*

_{i}*5 q*

*i*into Eq.~9! yields

*p** _{i}*5

*E*

_{ik}*q*

_{k}*~E**nl**q*_{l}*E*_{nm}*q** _{m}*!

^{1/2}, ~34!

where

*DE*_{ij}*Dt* 5 1

2~2v*ik*1lg^{˙}*ik**!E**kj*, ~35!

*and E** _{i j}* 5 d

*i j*initially@Bretherton ~1962!#.

* Since fibers in region dq are currently in region dp, the ODF becomes*
c

**~p! 5**c

_{0}

**~q!**

*dA*

_{q}*dA** _{p}* 5 c

_{0}

**~q!**

*~E*

*kl*

*q*

_{l}*E*

_{km}*q*

*!*

_{m}^{3/2}

det*~E** _{ij}*! 5c

_{0}

**~q!~L**

_{kl}*p*

*L*

_{l}

_{km}*p*

*!*

_{m}^{23/2}, ~36!

whereL*i j* *5 E*_{i j}^{21}.

From this, the second-order orientation tensor can be determined by @Altan and Rao

~1995!#

*a** _{ij}*5

### R

*S*

*p*_{i}*p** _{j}*c

**~p!dA***5*

_{p}### R

*S*

*E*_{ik}*q*_{k}*E*_{jk}*q*_{l}

*E*_{mn}*q*_{n}*E*_{mo}*q** _{o}*c

_{0}

**~q!dA***. ~37!*

_{q}**B. Numerical solution by the finite-element method**

*When C** _{I}*Þ 0, since an analytic solution is not available, the finite-element method
was applied to solve the ODF numerically. Rearranging Eq.~10! with the use of Eq. ~9!

yields a differential equation of the ODF in the form of
*D*c

*Dt* 5 2 ]

]^{p}*i*

### S

^{c}

^{p˙}

^{i}

^{h}

^{2D}

^{r}^{]}

^{]c}

^{p}

^{i}### D

^{,}

^{~38!}

where

*p˙*_{i}* ^{h}*5 2

^{1}2v

*ij*

*p*

*1*

_{j}^{1}2l~g

^{˙}

_{ij}

^{p}*2g*

_{j}

^{˙}

_{kl}

^{p}

_{k}

^{p}

_{l}

^{p}*!. ~39!*

_{i}Multiplying both sides of Eq.~38! by the arbitrary functionc*¯ and integrating over S, with*
special consideration of the gradient operator, yields

### R

*S*c

*c*

^{¯}^{D}*Dt* *dA*5

### R

*S*

]c^{¯}

]^{p}*i*

### S

^{c}

^{p˙}

^{i}

^{h}

^{2D}

^{r}^{]}

^{]c}

^{p}

^{i}### D

^{dA.}^{~40!}

Discretizing Eq. *~40! with triangular elements, whose shape functions are N*_{a}**(p) (**a
5 1,2,3), yields

*m*_{ab}
*D*c_{b}

*Dt* *5 k*_{ab}c_{b}~a^{,}b5 1,2,3!, ~41!

where

*m*_{ab}5

### R

*S*

*N*_{a}*N*_{b}*dA,* ~42!

*k*_{ab}5

### R

*S*

]^{N}_{a}

]^{p}*i*

### S

^{N}^{b}

^{p˙}

^{i}

^{h}

^{2D}

^{r}^{]}

^{]}

^{N}^{p}^{b}

^{i}### D

^{dA.}^{~43!}

**Representing the three nodal points of a triangular element ‘‘e’’ by p**^{1}**, p**^{2}**, and p**^{3}, the
shape functions can be defined as

*N*_{1}**~p! 5 ~p**^{23}**3p**^{31}**!3p**^{23}**•~p2p**^{2}*!/4A*^{2} **[ c**1* •p1d*1,

*N*_{2}**~p! 5 ~p**^{31}**3p**^{12}**!3p**^{31}**•~p2p**^{3}*!/4A*^{2} **[ c**_{2}* •p1d*2, ~44!

*N*_{3}**~p! 5 ~p**^{12}**3p**^{23}**!3p**^{12}**•~p2p**^{1}*!/4A*^{2} **[ c**_{3}* •p1d*3,

**where, p**^{ab}**5 p**^{b}**2p**^{a} *and A is the area of the triangular region*V*e**. From this, m*_{ab}and
*k*_{ab} can be derived as

*m*_{ab}5

### R

_{V}

_{e}

^{~c}^{a}

^{•p1d}^{a}

^{!~c}^{b}

^{•p1d}^{b}

^{!dA,}^{~45!}

*k*_{ab}5

### R

_{V}

_{e}

^{~c}^{a}

^{•p˙}

^{h}

^{!~c}^{b}

^{•p1d}^{b}

^{!dA2D}

^{r}### R

_{V}

_{e}^{$}

^{~c}^{a}

^{•c}^{b}

^{!2~c}^{a}

^{•p!~c}^{b}

^{•p!}^{%}

^{dA.}^{~46!}

For numerical calculations, the surface of a unit sphere was discretized by 2700 triangular
elements and the backward time derivative was employed with a time step of approxi-
mately*Dt 5 0.1/*g*˙ to ensure stability.*

**V. RESULTS AND DISCUSSION**

In order to determine appropriate FAC values for the modified hybrid model II and to examine the validity of the proposed closure approximations, orientation calculations were performed for homogeneous flows. Calculations were also performed for nonhomo- geneous flow fields to test the stability and generality of the current approximations.

*Since Folgar and Tucker’s model D*_{r}*5 C** _{I}*g

*˙ prevents relaxation of fiber orientation,*calculation of the fiber orientation in start-up flow is considered in the present investiga- tion. In all calculations, slender fibers (l 5 1) with initial random orientations were assumed.

**A. Determination of FAC**

Since the right side of governing Eq.~11! is a first degree homogeneous function of the velocity gradient, the time and velocity gradient can, respectively, be nondimension- alized as

*t*

### *

_{5 Gt and}### S

^{]}

^{]}

^{v}^{x}

^{i}

^{j}### D ^{*}

^{5}

^{G}^{1}

^{]}

^{]}

^{v}^{x}

^{i}

^{j}^{,}

^{~47!}

*where, G represents an arbitrary constant of dimension t*^{21}.

In this investigation, calculations were made using these nondimensionalized variables
and five representative flow fields were selected for the verification study as shown in
Table II*@Cintra and Tucker ~1995!#, where v**i**/G is shown. Calculations of the orienta-*
*tion tensor were performed for C** _{I}* values ranging from 0 to 0.1 with the closure approxi-
mations as summarized in Table III.

For simple shear flow ~SS!, model I and ORS were applied directly to the exact
*solution of a*_{i j}*to estimate b*_{i j kl}*and compared with the exact solutions of b** _{i j kl}*as shown
in Fig. 4. The comparison in Fig. 4

*~a! when C*

*I*5 0 shows that the exact solution lies

*between the results of model I and ORS for the entire region. When C*

*5 0.1, the comparison in Fig. 3~b! shows the same trend, but the exact solution can be seen to be closer to the results of model I. Similar trends could be observed for other flow fields and*

_{I}*other C*

*values. Such results show that the assumed parametric forms of C*

_{I}^{model I}and C

^{ORS}act as the lower and upper bounds, respectively, and therefore, it was construed that a combination of model I and ORS, if properly interpolated, would provide improved results.

To find the appropriate FAC for model II, numerical simulations were performed for
all five flow fields with an assumed FAC value. The root-mean-square errors of all the
*nonzero components of b** _{i j kl}*were calculated for each flow field and the FAC was chosen
to minimize the sum of those five or four error values depending on the amount of

*deviation. In Table IV, the determined FAC values are shown for selected C*

*values.*

_{I}*From these values, the FAC was approximated as a function of C** _{I}* as

FAC*5 0.5220.9655•C*_{I}^{1/2} *~0 , C**I* , 0.1!. ~48!

**TABLE II. Five representative flow fields for the verification study**@Cin-
tra and Tucker~1995!#.

Flow field Velocity field (v_{1}*/G,v*_{2}*/G,v*_{3}*/G)*

SS~simple shear! *(x*_{2},0,0)

SSA~shearing/stretching A! (*2x*1*110x*2,*2x*2*,2x*_{3})
SSB~shearing/stretching B! (*2x*1*1x*2,*2x*2*,2x*_{3})
UE~uniaxial elongation! *(2x*_{1},*2x*2,*2x*3)
BE~biaxial elongation! *(x*_{1}*,x*_{2},22x3)

**TABLE III. Summary of closure approximations used in the current in-**
vestigation.

Closure approximation Source

HYB~hybrid! Advani and Tucker~1987!, Eq. ~12!

ORS~orthotropic smooth! Cintra and Tucker~1995!, Eq. ~28!

ORF~orthotropic fitted! Cintra and Tucker~1995!

Model I~modified hybrid model I! Eq.~27!

Model II~modified hybrid model II! Eq. ~33!

**B. Homogeneous flow fields**

Comparisons of the calculation results using the five closure approximations as listed
in Table II and the exact values are shown in Figs. 5~a! and 5~b! for the case of simple
*shear flow with C*_{I}*5 0 and C**I* 5 0.01, respectively. It can be seen that model II out-
performs HYB, ORS, and model I as expected and nearly reproduces the exact values. It
can be seen in Fig. 5~b! that model II and ORF make better predictions than the other

**FIG. 4. Comparisons of b*** _{i j kl}*between the exact solution and approximate values for a simple shear flow with

*~a! C**I**5 0 and ~b! C**I*5 0.1.

**TABLE IV. FAC values determined for selected C*** _{I}*values.

*C** _{I}* 0.0 0.001 0.01 0.1

FAC 0.52 0.49 0.42 0.22

closure approximations both transiently and steadily, while in Fig. 5~a! ORF can be seen to deviate from the exact value as time increases, indicating the beginning of oscillation.

*Also, model I can be seen to give better results than the HYB when C** _{I}*5 0, but oscil-

*lation occurs when C*

*5 0.01.*

_{I}*For the simple shear flow, calculation results with different C** _{I}* values, namely, 0.001
and 0.1 are shown in Figs. 6~a! and 6~b!, respectively. Only the ORF and model II are
compared to the exact solution in Figs. 6

*~a! and 6~b!. The results show that when C*

*5 0.001, both the ORF and model II accurately follow the exact solution initially, but as time increases, model II has a maximum error of about 0.1 while the ORF starts to*

_{I}*oscillate with a magnitude 0.15. Further calculations after t*

### *

5 40 revealed that model II also oscillates for some time but with a smaller magnitude that eventually becomes*steady. When C*

*5 0.1, Fig. 6~b! shows that both the ORF and model II accurately predict the exact solution.*

_{I}**FIG. 5. Comparisons of a*** _{i j}*between the exact solution and simulations based on various closure approxima-
tions for simple shear flow with

*~a! C*

*I*

*5 0 and ~b! C*

*I*5 0.01.

*Poor performance of the ORF at low C** _{I}* values is due to the fact that the ORF was

*obtained from the exact solution when C*

*5 0.01. Thus, the fiber orientation prediction*

_{I}*becomes inaccurate for other values of C*

*. If the ORF was obtained by fitting the ODF*

_{I}*at various C*

*values, then this specific error might decrease, but the overall error for the general cases would most probably grow.*

_{I}For a quantitative measure of the errors, the concept of average and steady errors was employed@Cintra and Tucker ~1995!#. In this method, the scalar magnitude of errors at a given time is defined as follows:

*e*5

### A

*~e*

*i j*

*e*

_{i j}*!/2, where e*

_{i j}*5 a*

_{i j}^{exact}

*2a*

_{i j}^{closure}. ~49!

The average and steady errors using the various closure approximations for the five
*homogeneous flow fields are summarized in Table V. For C** _{I}*5 0.0 and 0.001, the ORF
shows oscillation behavior making the error values meaningless. Model II is very accu-

**FIG. 6. Comparisons of a*** _{i j}*between the exact solution and simulations based on various closure approxima-
tions for simple shear flow with

*~a! C*

*I*

*5 0.001 and ~b! C*

*I*5 0.1.

rate compared to the hybrid closure approximation for all cases and is equally or more
*accurate than the ORF depending on the C** _{I}*value. The only exception is the case of SSA

*at C*

*5 0.01, where model II is less accurate than the ORF.*

_{I}The results show that the HYB has some transient and steady-state errors, but it is a
very stable approximation that never behaves nonphysically. Also, calculation by the
HYB quickly reaches the steady state, which corresponds to a more aligned orientation
*state. The ORF can be seen to be more accurate than the HYB for C** _{I}*5 0.01, but for

*lower values of C*

*the errors increase drastically. Thus, overall, it can be concluded that*

_{I}*model II offers accurate solutions for a wide range of C*

*values.*

_{I}**C. Nonhomogeneous flow fields**

The first verification of fiber orientation calculations using the current closure approxi- mations in nonhomogeneous flow fields was performed in the combined flow field rep- resented by the following nondimensionalized velocity gradients @Cintra and Tucker

~1995!#:

### F

^{]}

^{]}

^{v}^{x}

^{i}

^{j}### G ^{*}

^{5}

### F

^{0}

^{0}

^{0}

^{1}

^{0}

^{0}

^{0}

^{0}

^{0}

### G

^{for}

^{0}

^{< t}^{*}

^{, 10,}

^{~50!}

### F

^{]}

^{]}

^{v}^{x}

^{i}

^{j}### G ^{*}

^{5}

^{20}

^{1}

### F

^{21}

^{0}

^{0}

^{21}

^{0}

^{0}

^{20}

^{0}

^{2}

### G

^{for}

^{10}

^{< t}^{*}

^{, 20,}

^{~51!}

**TABLE V. Average** ~avg! and steady ~std! errors between orientation tensor computations using various
closure approximations and exact solutions for homogeneous flow fields.

*C** _{I}* Flow

HYB ORF Model II

avg std avg std avg std

SS 0.050 0.023 0.134 0.070 0.005 0.005

SSA 0.094 0.046 0.033 0.027 0.015 0.002

0.0 SSB 0.058 0.021 0.008 0.009 0.007 0.004

UE 0.053 0.015 0.009 0.015 0.008 0.002

BE 0.011 0.001 0.002 0.001 0.004 0.001

SS 0.103 0.115 0.055 0.022 0.039 0.053

SSA 0.068 0.006 0.034 0.003 0.014 0.010

0.001 SSB 0.034 0.003 0.008 0.004 0.004 0.002

UE 0.031 0.003 0.009 0.005 0.004 0.002

BE 0.010 0.001 0.003 0.002 0003 0.001

SS 0.132 0.159 0.024 0.026 0.029 0.029

SSA 0.057 0.034 0.013 0.015 0.030 0.037

0.01 SSB 0.035 0.003 0.004 0.002 0.006 0.010

UE 0.032 0.003 0.004 0.004 0.005 0.008

BE 0.013 0.006 0.003 0.004 0.003 0.003

SS 0.050 0.060 0.007 0.009 0.006 0.008

SSA 0.023 0.026 0.005 0.006 0.003 0.004

0.1 SSB 0.073 0.077 0.024 0.036 0.004 0.002

UE 0.070 0.072 0.025 0.038 0.004 0.002

BE 0.022 0.025 0.004 0.006 0.002 0.003

### F

^{]}

^{]}

^{v}^{x}

^{i}

^{j}### G ^{*}

^{5}

^{1}

^{2}

### F

^{2}

^{0}

^{0}

^{21}

^{0}

^{0}

^{21}

^{0}

^{2}

### G

^{for}

^{20}

^{< t}^{*}

^{< 30.}

^{~52!}

The second test was performed for a center-gated disk flow in which the velocity field and velocity gradient are, respectively, given as follows:

*v** _{r}*5

*3Q*

8p*•rb*

### S

^{1}

^{2}

^{b}^{z}^{2}

^{2}

### D

^{5}

### S

^{8}

^{p}

^{3Q}^{•b}^{2}

### D

^{r}^{1}

^{*}

^{@12~z}^{*}

^{!}

^{2}

^{#, v}^{u}

^{5 v}

^{z}^{5 0,}

^{~53!}

### F

^{]}

^{]}

^{v}^{x}

^{i}

^{j}### G

^{5}

### S

^{8}

^{p}

^{3Q}^{•b}^{3}

### D

^{~r}^{*}

^{1}

^{!}

^{2}

### F

^{2@12~z}^{0}

^{0}

^{*}

^{!}

^{2}

^{#}

^{@12~z}^{0}

^{0}

^{*}

^{!}

^{2}

^{#}

^{22r}^{0}

^{0}

^{*}

^{z}^{*} G

^{,}

^{~54!}

*where, Q and b are the volume flow rate and half-gap thickness, respectively, with r*

### *

*5 r/b and z*

### *

*5 z/b. For simplification, the velocity field and time were nondimen-*

*sionalized with the factor 3Q/8*p

^{b}^{3}

*as the constant G in Eq.*~47!.

The detailed procedure for solving the orientation tensor in the center-gated disk flow
is available in the literature@Altan and Rao ~1995!#. In this study, the orientation tensors
*were calculated along the r direction at z*

### *

5 0.2, 0.5, and 0.7.The errors induced by the HYB, ORF, and model II in combined and center-gated disk
flows are summarized in Table VI. As can be seen in Table VI, the results are similar to
the case of homogeneous flows. As before, model II is more accurate than the HYB. The
*ORF oscillates when C** _{I}*5 0 or 0.001, and model II gives nearly the same results as the

*ORF when C*

*5 0 or 0.01. The maximum error based on model II in the case of the*

_{I}*combined flow occurred when C*

*5 0.01, while for the center-gated disk flow it oc-*

_{I}**TABLE VI. Average**~avg! and maximum ~max! errors between orientation tensor computations using various
closure approximations and exact solutions for nonhomogeneous flow fields.

*C** _{I}* Flow

HYB ORF Model II

avg max avg max avg max

0.0

Combined 0.078 0.206 0.026 0.066 0.005 0.015

*Disk (z**_{5 0.2)} 0.110 0.116 0.016 0.056 0.008 0.013

*Disk (z**5 0.5) 0.061 0.063 0.217 0.348 0.015 0.017

*Disk (z**5 0.7) 0.039 0.040 0.385 0.513 0.014 0.015

0.001

Combined 0.086 0.172 0.030 0.067 0.024 0.052

*Disk (z**5 0.2) 0.097 0.118 0.042 0.141 0.005 0.009

*Disk (z**5 0.5) 0.075 0.145 0.219 0.364 0.045 0.078

*Disk (z**5 0.7) 0.151 0.219 0.245 0.332 0.063 0.093

0.01

Combined 0.086 0.154 0.017 0.045 0.025 0.063

*Disk (z**5 0.2) 0.064 0.112 0.028 0.050 0.009 0.019

*Disk (z**5 0.5) 0.103 0.179 0.013 0.021 0.029 0.034

*Disk (z**_{5 0.7)} 0.143 0.177 0.018 0.026 0.029 0.040

0.1

Combined 0.067 0.096 0.014 0.028 0.008 0.021

*Disk (z**5 0.2) 0.039 0.064 0.009 0.011 0.006 0.007

*Disk (z**_{5 0.5)} 0.046 0.056 0.009 0.010 0.007 0.008

*Disk (z**5 0.7) 0.052 0.058 0.010 0.010 0.008 0.009

*curred at z*

### *

*5 0.7 with C*

*5 0. These two cases are shown in Fig. 7, and as can be seen, although the error values are maximum, model II tracks the variation reasonably well for both cases.*

_{I}**D. Contribution to extra stress**

In the above verification tests, the flow fields were assumed to be independent of the fiber orientation. However, in reality extra stress is induced by the fiber orientation.

Therefore, it must be checked whether the extra stress can be predicted accurately using the proposed closure approximations.

Considering the effects of fiber orientation, the stress equation can be written in the following form@Tucker ~1991!#

t*ij*5h*s*g^{˙}*ij*1h*s**c*$* ^{A}*g

^{˙}*kl*

*a*

_{ijkl}*1B~*g

^{˙}*ik*

*a*

_{kj}*1a*

*ik*g

^{˙}*kj*

*!1C*g

^{˙}*ij*

*12Fa*

*ij*

*D*

*%*

_{r}^{,}~55!

**FIG. 7. Comparisons of a*** _{i j}*between the exact solution and simulations based on the HYB; ORF, and model II
for

*~a! combined flow with C*

*I*

*5 0.01 and ~b! center-gated disk flow at z**

*5 0.7 with C*

*I*5 0.001.

whereh*s**is the solvent viscosity, c is the particle volume fraction, and A, B, C, and F are*
material constants. Since the fitting procedure used to obtain model II involved minimiz-
*ing the errors of a*_{i jkl}*and model II was found to accurately predict a** _{i j}*, it is construed
that the extra stress can be accurately predicted by using model II in solving the orien-
tation tensor.

For example, in the coupled lubrication region, Eq.~55! can be simplified as
t_{2}_{a}5h*s*g^{˙}_{2}_{a}12h*s**N** _{p}*$g

*12*

^{˙}*a*

_{2}

_{a}

_{12}1g

^{˙}_{32}

^{a}_{2}

_{a}

_{32}% ~a 5 1,3!, ~56!

*where N** _{p}* is the material constant and the subscript 2 denotes the thickness direction. If

*simple shear flow is assumed in this case, the ratio of the extra stress becomes 2N*

_{p}*a*

_{2112}.

*The comparisons of a*

_{2112}between the exact solution and simulations based on the HYB,

*ORF, and model II for SS flow with C*

*5 0.001 and 0.01 are shown in Figs. 8~a! and*

_{I}**FIG. 8. Comparisons of a**_{2112}, which denotes the contribution of extra stress induced by fiber orientation in
total stress, between the exact solution and simulations based on various closure approximations for simple
shear flow with*~a! C**I**5 0.001 and ~b! C**I*5 0.1.